LMucko/crystallography-open-database huggingface dataset:
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on heating T = 581 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003595
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on heating T = 581 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.44082
_cell_formula_units_Z            8
_cell_length_b                   8.44082
_cell_length_c                   8.44082
_cell_volume                     601.387
_database_code_amcsd             0003688
_diffrn_ambient_temperature      854.15
_exptl_crystal_density_diffrn    4.418
_exptl_crystal_thermal_history   'heating T = 581 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003595
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on heating T = 601 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003596
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on heating T = 601 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.44366
_cell_formula_units_Z            8
_cell_length_b                   8.44366
_cell_length_c                   8.44366
_cell_volume                     601.994
_database_code_amcsd             0003689
_diffrn_ambient_temperature      874.15
_exptl_crystal_density_diffrn    4.413
_exptl_crystal_thermal_history   'heating T = 601 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003596
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on heating T = 658 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003597
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on heating T = 658 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.44737
_cell_formula_units_Z            8
_cell_length_b                   8.44737
_cell_length_c                   8.44737
_cell_volume                     602.788
_database_code_amcsd             0003690
_diffrn_ambient_temperature      931.15
_exptl_crystal_density_diffrn    4.408
_exptl_crystal_thermal_history   'heating T = 658 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003597
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on heating T = 696 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003598
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on heating T = 696 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.45225
_cell_formula_units_Z            8
_cell_length_b                   8.45225
_cell_length_c                   8.45225
_cell_volume                     603.833
_database_code_amcsd             0003691
_diffrn_ambient_temperature      969.15
_exptl_crystal_density_diffrn    4.400
_exptl_crystal_thermal_history   'heating T = 696 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003598
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on heating T = 753 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003599
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on heating T = 753 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.45830
_cell_formula_units_Z            8
_cell_length_b                   8.45830
_cell_length_c                   8.45830
_cell_volume                     605.131
_database_code_amcsd             0003692
_diffrn_ambient_temperature      1026.15
_exptl_crystal_density_diffrn    4.390
_exptl_crystal_thermal_history   'heating T = 753 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003599
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on heating T = 791 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003600
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on heating T = 791 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.46018
_cell_formula_units_Z            8
_cell_length_b                   8.46018
_cell_length_c                   8.46018
_cell_volume                     605.534
_database_code_amcsd             0003693
_diffrn_ambient_temperature      1064.15
_exptl_crystal_density_diffrn    4.388
_exptl_crystal_thermal_history   'heating T = 791 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003600
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on heating T = 848 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003601
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on heating T = 848 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.46608
_cell_formula_units_Z            8
_cell_length_b                   8.46608
_cell_length_c                   8.46608
_cell_volume                     606.802
_database_code_amcsd             0003694
_diffrn_ambient_temperature      1121.15
_exptl_crystal_density_diffrn    4.378
_exptl_crystal_thermal_history   'heating T = 848 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003601
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on heating T = 906 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003602
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on heating T = 906 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.47175
_cell_formula_units_Z            8
_cell_length_b                   8.47175
_cell_length_c                   8.47175
_cell_volume                     608.022
_database_code_amcsd             0003695
_diffrn_ambient_temperature      1179.15
_exptl_crystal_density_diffrn    4.370
_exptl_crystal_thermal_history   'heating T = 906 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003602
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on heating T = 944 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003603
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on heating T = 944 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.47516
_cell_formula_units_Z            8
_cell_length_b                   8.47516
_cell_length_c                   8.47516
_cell_volume                     608.757
_database_code_amcsd             0003696
_diffrn_ambient_temperature      1217.15
_exptl_crystal_density_diffrn    4.364
_exptl_crystal_thermal_history   'heating T = 944 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003603
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on heating T = 982 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003604
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on heating T = 982 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.47670
_cell_formula_units_Z            8
_cell_length_b                   8.47670
_cell_length_c                   8.47670
_cell_volume                     609.089
_database_code_amcsd             0003697
_diffrn_ambient_temperature      1255.15
_exptl_crystal_density_diffrn    4.362
_exptl_crystal_thermal_history   'heating T = 982 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003604
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 963 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003605
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 963 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.47405
_cell_formula_units_Z            8
_cell_length_b                   8.47405
_cell_length_c                   8.47405
_cell_volume                     608.517
_database_code_amcsd             0003698
_diffrn_ambient_temperature      1236.15
_exptl_crystal_density_diffrn    4.366
_exptl_crystal_thermal_history   'cooling T = 963 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003605
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 944 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003606
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 944 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.47392
_cell_formula_units_Z            8
_cell_length_b                   8.47392
_cell_length_c                   8.47392
_cell_volume                     608.489
_database_code_amcsd             0003699
_diffrn_ambient_temperature      1217.15
_exptl_crystal_density_diffrn    4.366
_exptl_crystal_thermal_history   'cooling T = 944 C'
_cod_original_cell_volume        608.490
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003606
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 906 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003607
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 906 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.47029
_cell_formula_units_Z            8
_cell_length_b                   8.47029
_cell_length_c                   8.47029
_cell_volume                     607.708
_database_code_amcsd             0003700
_diffrn_ambient_temperature      1179.15
_exptl_crystal_density_diffrn    4.372
_exptl_crystal_thermal_history   'cooling T = 906 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003607
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 848 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003608
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 848 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.46438
_cell_formula_units_Z            8
_cell_length_b                   8.46438
_cell_length_c                   8.46438
_cell_volume                     606.437
_database_code_amcsd             0003701
_diffrn_ambient_temperature      1121.15
_exptl_crystal_density_diffrn    4.381
_exptl_crystal_thermal_history   'cooling T = 848 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003608
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 791 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003609
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 791 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.46211
_cell_formula_units_Z            8
_cell_length_b                   8.46211
_cell_length_c                   8.46211
_cell_volume                     605.949
_database_code_amcsd             0003702
_diffrn_ambient_temperature      1064.15
_exptl_crystal_density_diffrn    4.385
_exptl_crystal_thermal_history   'cooling T = 791 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003609
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 753 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003610
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 753 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.45708
_cell_formula_units_Z            8
_cell_length_b                   8.45708
_cell_length_c                   8.45708
_cell_volume                     604.869
_database_code_amcsd             0003703
_diffrn_ambient_temperature      1026.15
_exptl_crystal_density_diffrn    4.392
_exptl_crystal_thermal_history   'cooling T = 753 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003610